Graphitic Carbon Nitride: Synthesis, Properties, and Applications in Catalysis Junjiang Zhu,*,† Ping Xiao,† Hailong Li,† and Sónia A. C. Carabineiro‡ †
Key Laboratory of Catalysis and Materials Science of the State Ethnic Aﬀairs & Commission Ministry of Education, South-Central University for Nationalities, Wuhan 430074, China ‡ Laboratory of Catalysis and Materials (LCM), Associate Laboratory (LSRE/LCM), Department of Chemical Engineering, Faculty of Engineering, University of Porto, Rua Dr. Roberto Frias, 4200-465 Porto, Portugal ABSTRACT: Graphitic carbon nitride, g-C3N4, is a polymeric material consisting of C, N, and some impurity H, connected via tris-triazine-based patterns. Compared with the majority of carbon materials, it has electron-rich properties, basic surface functionalities and H-bonding motifs due to the presence of N and H atoms. It is thus regarded as a potential candidate to complement carbon in material applications. In this review, a brief introduction to g-C3N4 is given, the methods used for synthesizing this material with diﬀerent textural structures and surface morphologies are described, and its physicochemical properties are referred. In addition, four aspects of the applications of g-C3N4 in catalysis are discussed: (1) as a base metal-free catalyst for NO decomposition, (2) as a reference material in diﬀerentiating oxygen activation sites for oxidation reactions over supported catalysts, (3) as a functional material to synthesize nanosized metal particles, and (4) as a metal-free catalyst for photocatalysis. The reasons for the use of gC3N4 for such applications are also given, and we expect that this paper will inspire readers to search for further new applications for this material in catalysis and in other ﬁelds. KEYWORDS: graphitic carbon nitride, synthesis, physicochemical properties, applications, metal-free catalyst, reference material, functional material
Figure 1. Multiple surface functionalities found on g-C3N4. Reprinted with permission from ref 5. Copyright 2008 Royal Society of Chemistry.
inducing Lewis-base character toward metal-free coordination chemistry and catalysis. Because of the presence of hydrogen and tothe fact that nitrogen has one more electron than carbon, g-C3N4 has rich surface properties that are important to catalysis, such as basic surface functionalities, electron-rich properties, H-bonding Received: May 13, 2014 Accepted: September 12, 2014 Published: September 12, 2014 16449
Figure 2. XRD patterns of g-C3N4 synthesized from cyanamide at diﬀerent temperatures. (A) Cyanamide was used as received. Reprinted with permission from ref 5. Copyright 2008 Royal Society of Chemistry. (B) Cyanamide was pretreated with a NaOH solution.
but may lead to diﬀerences in the product yield, degree of condensation and, especially, surface properties, which will be described in detail in the following section. In order to promote the condensation process and lower the condensation temperature, the synthesis should be conducted in a basic environment. Pure g-C3N4 is obtained at ca. 500 °C when the precursor cyanamide is pretreated with a basic solution (like aqueous NaOH), as conﬁrmed by XRD (Figure 2B). This indicates that the presence of hydroxyl ions facilitates the transformation of cyanamide to g-C3N4, probably due to the hydroxyl ions that promote the condensation process, by reacting with the hydrogen atoms on the edges of the intermediate. The reduction of the condensation temperature promotes some properties, like the surface area of the material, because of less aggregation. However, cyanamide is expensive and explosive,24,25 and the solubility of its derivates (dicyanamide or melamine) is low, therefore the synthesis of g-C3N4 with the desired (e.g., porous) structures, using these precursors, is either expensive or hard to operate. To overcome this limitation, Xu et al. reported the use of guanidine hydrochloride (GndCl), which is a water-soluble, environmentally friendly, and cheap material, as a precursor, to synthesize g-C3N4.25 They found that the material can be produced by direct condensation of the GndCl in Ar atmosphere at 550 °C for 3 h, which is similar to the procedure operated using cyanamide as precursor. Similar to that reported for cyanamide, the condensation of GndCl occurs by the transformation of melamine to melem, polymeric melem, and ﬁnally to g-C3N4, with subsequent release of NH3. The surface area of g-C3N4 prepared by direct polycondensation of C-, N-, and H-containing precursors is normally low (ca. 10 m2/g),8 because of the graphitic layered structure. This limits the performances of g-C3N4 in heterogeneous catalysis, since surface reactions require the catalyst to exhibit a certain surface area, to adsorb and activate the substrate. In order to overcome this limitation, g-C3N4 can be deposited on a high surface area material, like SBA-15.27 As g-C3N4 is a polymeric material, it can coat or spread on the support surface forming a ﬁlm layer with increased surface area. Wang et al. reported that Fe incorporated g-C3N4 (Fe-g-C3N4) can be homogeneously coated on SBA-15 (Figure 3) by an impregnation method, with a surface area increase from 8 to 506 m2/g.26 The activity raised from 0 (for Fe-g-C3N4) to 15 h−1 (for Fe-g-C3N4/SBA-15), in terms of TOF, for the photocatalytic oxidation of benzene to
motifs, etc., as shown in Figure 1. Moreover, its high thermal stability (it is stable up to 600 °C in air)7 and hydrothermal stability (it is insoluble either in acidic, neutral or basic solvents)8 enables the material to function either in liquid or gaseous environments, and at elevated temperatures, potentiating its wide applications in heterogeneous catalysis. Indeed, it has been reported that g-C3N4 is a promising catalyst for various reactions, including CO2 activation,9,10 transesteriﬁcation,11 oxygen reduction,12,13 hydrogen production,8,14−16 photodegradation of dyes,17 etc. Several reviews reporting the catalytic performances of g-C3N4 in a variety of reactions can be found elsewhere.4,18−21 This work overviews the recent advances of g-C3N4 in three aspects, based on the results obtained by the authors, as well as those from literature: (1) comparison of the reported preparation methods by a condensation route; (2) discussion of the thermal behavior and surface basicity of materials prepared using diﬀerent conditions; (3) description of several interesting uses of g-C3N4 in catalysis, already reported by the authors and in the literature, and the reasons why g-C3N4 has been used for such applications. This review also aims to provide basic knowledge in the synthesis of g-C3N4 samples with diﬀerent properties and inspire the readers to seek new applications of these materials in catalysis or material sciences.
2. SYNTHESIS The most common precursors used for chemical synthesis of gC3N4 are reactive nitrogen-rich and oxygen-free compounds containing prebonded C−N core structures, such as triazine and heptazine derivatives, most of them being unstable, diﬃcult to obtain and/or highly explosive. The synthesis of single-phase sp3-hybridized carbon nitrides is a challenging task due to their low thermodynamic stability.22,23 Not surprisingly, it seems that the defect materials are much more valuable than the ideal one, in particular for catalysis, which requires surface defects. Thus, the synthesis of g-C3N4 with defects is an interesting topic, when the material is going to be used in catalysis. The condensation pathways from cyanamide to Dicyandiamide, and to melamine and all other C/N materials are simple and good synthetic routes to generate slightly defected polymeric species.5 The cyanamide precursor is ﬁnally transformed to g-C3N4 at ca. 550 °C, as conﬁrmed by XRD (Figure 2A), with consequent formation of NH3. The synthesis can be conducted either in inert (e.g., N2, Ar) or in air atmosphere, with no signiﬁcant changes in the bulk structure; 16450
instead of yellow. The preparation of porous g-C3N4 with structured (like SBA-15) and soft templates are illustrated in a previous review article.19 The successful fabrication of g-C3N4 using diﬀerent templates makes possible to synthesize materials with the desired porous structures and surface morphologies, for speciﬁc uses. Oxygen-containing materials can also be used as precursors to produce g-C3N4. Dong et al. report that heating urea in a muﬄe furnace in the range of 450−600 °C for 2 h, with a heating rate of 15 °C min−1, results in the formation of gC3N4.33 In particular, the authors state that the heating temperature signiﬁcantly aﬀects the thickness and surface area of the resulting material, as shown in Figure 5. The layer
Figure 3. Typical TEM images of Fe-g-C3N4/SBA-15 and the corresponding elemental mapping images for C, N, and Fe.26 Reprinted with permission from ref 26. Copyright 2009 American Chemical Society Publishing.
phenol using H2O2 as oxidant, because of the increase in surface area and possibly the change in surface morphology. Another strategy, that is more eﬀective in improving the surface area, is to synthesize a material with porous structure using a template method, as illustrated in Figure 4A, which can
Figure 5. (A) TEM images of g-C3N4 synthesized at 450 and 575 °C using urea as precursor. (B) Dependence of the surface area of g-C3N4 on the treating temperature. Reprinted with permission from ref 33. Copyright 2011 Royal Society of Chemistry.
thickness decreases from 30 nm, for g-C3N4 synthesized at 450 °C (CN-450), to 20 nm, for the material synthesized at 575 °C (CN-575). Accordingly, the surface area increases from 12 m2/ g for CN-450 to 83 m2/g for CN-575. This is interesting, as high-surface-area g-C3N4 (up to ca. 97 m2/g) can be obtained by direct polycondensation without the use of a template. However, the formation mechanism is not yet clearly understood. Similarly to what is observed for cyanamide in Figure 2B, Zou et al. claim that the temperature for g-C3N4 formation, using urea as precursor, can be lowered to 300 °C when the synthesis is conducted on OH-rich mesoporous TiO2 spheres.34 They believe that the low temperature needed is due to the presence of −OH groups, and a mechanism regarding the role of these groups in the synthesis process is proposed, as depicted in Scheme 1, where titanol groups (Ti−OH) are used to attack the carbonyl of isocyanic acid (eq 2), to form Ti-NH2 groups, which subsequently react with cyanic acid to generate cyanamide (eq 3) and ﬁnally yield g-C3N4 (eq 4). Besides the above-mentioned methods, there are many other procedures described for the synthesis of g-C3N4 with diﬀerent surface morphologies and textural structures.35−37 Dai et al. report that g-C3N4 submicrospheres can be synthesized by a microwave method and that the prepared g-C3N4 has a surface area of up to 89.1 m2/g.35 There are several reviews5,19,38−40 that summarize the methods for the preparation of g-C3N4, with controllable morphology and structure. Those procedures are not mentioned in this work in order to avoid repetitions. Interested readers are referred to those publications.5,19,38−40
Figure 4. (A) Sketch for the preparation of porous g-C3N4 using a hard template. Reprinted with permission from ref 28. Copyright 2008 American Chemical Society. (B) TEM image of g-C3N4 replicated from SBA-15. Reprinted with permission from ref 29. Copyright 2009 John Wiley & Sons.
be seen as the result of removing the support from a g-C3N4support composite. Indeed, it is reported in the literature that porous g-C3N4 with an improved surface area can be prepared using Ludox HS40 Silica as a template and, more interestingly, the surface area and total pore volume of g-C3N4 can be controlled by simply adjusting the mass ratio of precursor to silica template.14 g-C3N4 materials with various structures and surface morphologies can be fabricated due to their polymeric properties, when appropriate templates are used.28,30 For instance, Jun et al. report that 2D g-C3N4 can be replicated from ordered mesoporous SBA-15, as shown in Figure 4B.29 Porous g-C3N4 can also be synthesized using surfactants (e.g., Triton X-100, P123, Brij 58) or ionic liquids as soft templates through a self-polymerization reaction.31,32 However, the ﬁnal product can be contaminated with residual carbon coming from the template polymers, which can easily be identiﬁed by the naked eye, as the obtained g-C3N4 is black, 16451
Scheme 1. Proposed Mechanism for the Formation of g-C3N4 Starting from Urea and Conducted on an OH-Rich TiO2 Supporta
Reprinted with permission from ref 34. Copyright 2011 Royal Society of Chemistry.
Figure 6. (A) TGA curves for g-C3N4 conducted in diﬀerent atmospheres. Reprinted with permission from ref 7. Copyright 2012 Elsevier Publishing. (B) TGA-MS spectra of g-C3N4 obtained at the temperature of 530 °C. Reprinted with permission from ref 41. Copyright 2009 Universitätsbibliothek Potsdam & MPI of Colloids and Interfaces.
3. PHYSICOCHEMICAL PROPERTIES Polymeric materials normally show low thermal stability and are readily oxidized (gasiﬁed) in oxidizing atmosphere, which makes them unsuitable as practical catalysts, especially for reactions conducted at high temperature ranges. In order to conﬁrm that g-C3N4 has suﬃcient thermal stability for catalytic use, thermal gravimetric analysis (TGA) measurements need to be performed, as they reﬂect the thermal behavior of materials and provide direct evidence of which temperature ranges the materials can endure. Figure 6A depicts the TGA curves of g-C3N4 obtained with diﬀerent conditions, showing that the material is stable up to 600 °C, either in N2, O2 or air atmosphere, and that the TGA curves obtained are similar.7 This suggests that g-C3N4 can endure high temperatures, even in oxidizing atmosphere, and the weight loss at above 600 °C is not due to the oxidation by O2 (to form oxides such as CO or CO2), but to the direct thermal decomposition of g-C3N4 itself. Combined TGA-MS results conﬁrm that the decomposition products contain mainly CNH, NH3 and C2N2 species, and that no oxide product is detected, as shown in Figure 6B.41 This shows that g-C3N4 is inert in oxygen atmosphere, otherwise the TGA proﬁles would be diﬀerent when N2 and O2 are used, and oxidized products would be formed. The high thermal stability demonstrates that
g-C3N4 can work for reactions conducted in oxidative atmosphere and at high temperatures. Due to its chemical inertness to molecular oxygen, it is expected that g-C3N4 can show interesting results in catalysis, unlike traditional inorganic materials that are reactive to molecular oxygen. g-C3N4 also shows good chemical stability in a variety of conventional solvents, including water, alcohols, dimethylformamide, tetrahydrofuran, diethyl ether and toluene, which makes it an excellent material, not only for gas-phase reactions conducted at elevated temperatures (as mentioned above), but also for liquid-phase reactions, carried out in various solvents. It is reported that no essential change in the IR spectra is observed for g-C3N4 after it is soaked in the above solutions for up to 30 days, conﬁrming its excellent stability and durability.18 However, exceptions are reported, when the material is treated in molten alkali metal hydroxides and concentrated acids.42 As demonstrated above, the replacement of C by N in the six-membered C−N−C rings produces surface basic groups on the g-C3N4 surface, which facilitates its use as a base catalyst. The importance of the surface basicity of g-C3 N4 is demonstrated in several reactions, including C−C coupling,43 α−C-H activation44 and NO decomposition.7 The surface basicity of g-C3N4 can be identiﬁed and evaluated by temperature-programmed desorption of CO2 (CO2-TPD), 16452
Figure 7. (A) CO2-TPD proﬁles of g-C3N4 synthesized under diﬀerent conditions; (B) peak deconvolution for the CO2-TPD proﬁle of gC3N4_H2O; (C) Possible basic sites used for CO2 adsorption on g-C3N4.
phosphor can improve the electric conductivity by 4 orders of magnitude and photocurrent generation by 5 orders of magnitude, compared to the pure g-C3N4.51 Many other interesting physicochemical properties of g-C3N4 are introduced and documented in other works.4,18−21 For space limitations and to avoid repetition they are not detailed in this review. Interested readers are referred to those publications. 4,18−21 It should be noted, however, that such modiﬁcations or functionalizations are very useful for changing the surface properties of g-C3N4, and are especially important concerning the optimization of its catalytic performance.
which is a powerful technique in measuring the surface basicity of materials. In several recent works, it is shown that covalent triazine frameworks (CTFs), which are a kind of carbon nitrides, exhibit good surface basicity and show excellent performances for the synthesis of cyclic and linear carbonates from CO2 and epoxides, as well as for dye removal by adsorption.45,46 Figure 7A depicts the CO 2 -TPD proﬁles of g-C 3 N 4 synthesized under diﬀerent conditions, which show a large amount of surface basic groups. It is known that there are three types of surface basic sites in which CO2 can be adsorbed on, namely: “N” in the C−N−C six-membered rings, and “ NH” and “−NH2” groups on the surface edges, as shown in Figure 7C, which result in three deconvoluted CO2 desorption peaks in the CO2-TPD proﬁle. The former two desorption peaks are clearly observed, whereas the latter appears above 300 °C and is overlapped, as shown in the TPD proﬁle. Although the XRD patterns show no change in the bulk structure, it was found that the surface basicity is signiﬁcantly aﬀected if g-C3N4 is synthesized in diﬀerent atmospheres. The sample prepared by thermal condensation of cyanamide, in nitrogen atmosphere, at 550 °C for 4 h (g-C3N4_N2), shows two desorption peaks at 145 and 297 °C, which become closer when the sample is synthesized in air atmosphere (g-C3N4_air). Moreover, only one CO2 desorption peak is found for gC3N4_H2O, prepared by ﬁrst dissolving the precursor cyanamide in aqueous solution and subsequently treated in air atmosphere. This desorption proﬁle can be deconvoluted into three peaks, in terms of the basic sites analyzed above, as shown in Figure 7B, and the temperature diﬀerence for the former two desorption peaks is closer. The shift in the desorption temperature suggests that the surface basic intensity of g-C3N4 is changed, which might be caused by the vapors in the environment, as the percentage of vapors found in the atmosphere increases from g-C3N4_N2 to g-C3N4_air and further to g-C3N4_H2O. It is reported that the vapors in the heating atmosphere facilitate the release of NH3 from nitrogen containing carbonaceous materials, and change the surface basicity of material,47,48 supporting the above results. Modiﬁcations or functionalizations of g-C3N4 are often carried out to widen its applications and discover its essential properties. Both in situ modiﬁcation and postfunctionalization are possible. g-C3N4 can be in situ doped with boron,44 ﬂuorine,49 sulfur,50 phosphor51 or protonated with HCl.42 That is well-documented and summarized in several reviews.4,18 Such modiﬁcations enhance the properties of the material and improve its applications. For example, the doping with
4. MULTIFUNCTIONAL APPLICATIONS IN CATALYSIS The applications of g-C3N4 in catalysis have been extensively investigated in recent years, and it is now established that gC3N4 is a good catalyst for a wide variety of reactions. In order to diﬀerentiate and avoid overlapping the contents of previous works, in this review, the applications of g-C 3 N 4 in heterogeneous catalysis are referred from three diﬀerent aspects, and the reasons for the use of this material in such applications is given. The ﬁrst point is the use of g-C3N4 as a metal-free catalyst for catalytic reactions (namely NO decomposition); the second is its use as a reference material, to diﬀerentiate the oxygen activation sites in oxidation reactions conducted on supported catalysts; and the third is its application as a high surface support with a large amount of functional groups, ideal to prepare small and stable metal nanoparticles (NPs). Also, the application of g-C3N4 in photocatalysis, one of the most current research topics worldwide, is described, based on the achievements mentioned in the literature. We expect that this work will inform the reader about the multifunctional properties of this exciting material and that will stimulate research to ﬁnd new applications in heterogeneous catalysis or other ﬁelds in the future. 4.1. As a Metal-Free Catalyst for NO Decomposition. Nitrogen monoxide (NO) is a hazardous pollutant that causes environmental problems, such as acid rain and urban smog, and its removal is a challenging task nowadays. 52 Direct decomposition of NO into N2 and O2 (2 NO → N2 + O2) is an ideal route for NO removal, as no reductant is needed and the products are the nontoxic N2 and O2. However, this reaction route is not yet carried out in industry since current inorganic catalysts encounter many problems when operating in real conditions. Another problem is that gaseous oxygen in the reacting atmosphere has negative eﬀects on the reaction, namely: (1) it suppresses the desorption of atomic oxygen (formed in NO dissociation) from the active sites, making their 16453
Figure 8. (A) Theoretical simulation of NO decomposition on g-C3N4 by density functional theory (DFT) calculation; (B) theoretic model for calculating the Mulliken charge distribution of NO before and after adsorption on g-C3N4. Reprinted with permission from ref 7. Copyright 2010 Royal Society of Chemistry.
The suitability of g-C3N4 to catalyze NO decomposition is conﬁrmed by the experimental results shown in Table 2, which
regeneration diﬃcult and thus poisoning the catalyst; (2) it competes with NO on the surface oxygen defects (active sites) during the adsorption process, preventing NO adsorption and activation on the catalyst surface and thus decreasing the activity.53,54 From the molecular orbital diagram of the NO molecule, (σ1s)2(σ1s*)2(σ2s)2(σ2s*)2(σ2p)2(π2p)4(π2p*)1, it is known that the bond order of N−O is 2.5, and can be lowered to 2.0, if NO gains an electron in the (π2p*) energy band, which favors the rupture of the N−O bond. Hence, an ideal NO decomposition catalyst should have weak interactions or be inert to oxygen, in order to avoid the negative eﬀects caused by this gas, and have electron-rich properties, so that it can donate electrons to NO and thus decrease the order of the N−O bond. g-C3N4 has strong resistance to oxygen and electron-rich properties (surface basic sites), being a suitable catalyst for NO decomposition. In addition, the polar C−N−C groups of gC3N4 can also provide ideal adsorption sites for NO (that is a polar molecule). In order to verify the applicability of g-C3N4 to NO decomposition, theoretical simulations based on density functional theory (DFT) calculations were attempted, showing that the N−O bond length can be elongated from 1.163 to 1.381 Å when NO is parallelly adsorbed on g-C3N4, as shown in Figure 8A, conﬁrming that g-C3N4 is a suitable catalyst for NO dissociation.7 To explain NO dissociation on g-C3N4, we calculated the Mulliken charge distributions of NO before and after adsorption on the material, as depicted in Figure 8B and Table 1, showing that the values varies from 0 for the free NO
Table 2. NO Conversion over Several g-C3N4-Based Catalysts at Diﬀerent Temperatures.7 NO conversion (%) at diﬀerent temperatures
g-C3N4 g-C3N4a Zn-g-C3N4 Pt-g-C3N4 Au-g-C3N4
0.14 2.14 10.83 7.46 26.88
3.46 18.58 32.37 19.92 23.01
5.03 33.33 48.31 35.65 26.59
15.06 46.25 69.40 49.61 41.05
g-C3N4 synthesized in basic medium before calcination
demonstrate that g-C3N4 is active for NO decomposition at temperatures above 400 °C, and that the activity increases with temperature, in accordance with the DFT calculations. The activity can be further increased when metal ions (e.g., Na+, Zn2+, Au, etc.) are incorporated into the framework. Very interestingly, the incorporation of zinc (i.e., Zn-g-C3N4) leads to similar or even better NO decomposition activities, compared to noble metals (e.g., Pt-g-C3N4). Considering that Zn is inactive for NO decomposition, while Pt is active, the comparable activities observed for the Zn- and Pt- incorporated samples suggest that the metal in g-C3N4 is not the active site. This suggests that the surface basic sites of g-C3N4 are responsible for the activity, as indicated in DFT simulations (cf. Figure 8A). The excellent behavior of g-C3N4 for base reactions is well-documented in a recent paper by Li et al., based on a Schottky eﬀect.20 This result opens a new panorama to design low-cost (noble metal free), green, and environmentally friendly catalysts for NO decomposition. It is worth to point out that since g-C3N4 has a strong resistance to oxygen, the NO decomposition reaction thus can be conducted in the presence of this gas, without the negative eﬀects observed for inorganic catalysts. This makes g-C3N4 a very attractive catalyst, compared to others reported in the literature, and reinforces its potential role in NO decomposition in the future. 4.2. As a Reference Material to Diﬀerentiate O2 Activation Site. Catalytic oxidation is one of the most important reactions in industry and our daily life. Molecular oxygen is the preferred oxidant due to its easy availability, low cost and nontoxicity. As O2 molecule is not very active, it should be activated and dissociated into atomic oxygen before participating in the reaction.55 The pathway for oxygen activation is still under discussion, especially for reactions carried out on supported catalysts. Schubert et al. suggest three
Table 1. Mulliken Charge Distribution of Diﬀerent Atoms before and after the Adsorption of NO on g-C3N4a 7 after adsorption before adsorption
qN: The Mulliken charge of N atom of NO; qO: The Mulliken charge of O atom of NO; qNO: The Mulliken charge of NO; qCsub: The Mulliken charge of C atom of C3N4; qNsub: The Mulliken charge of N atom of C3N4
molecule to −0.271 when it is adsorbed, and the change in qO is more negative than that in qN.7 This shows that electrons are transferred from g-C3N4 to the NO molecule, and that the O atom of NO is connected to the basic sites of g-C3N4. These results explain why NO can be dissociated on g-C3N4 and suggest that g-C3N4 can catalyze NO decomposition (at least in theory). 16454
replacing that support by g-C3N4, and comparing the obtained activities. Figure 10A compares the catalytic performances of gold NPs supported on activated carbon (Au/AC) and g-C3N4 (Au/gC3N4) for the selective oxidation of benzyl alcohol using molecular oxygen as oxidant.64 The Au/AC catalyst shows 90.8% conversion for benzyl alcohol for reaction time of 3 h, while that obtained from the Au/g-C3N4 catalyst is only 5.7% even after 5 h. Considering that the adsorption and activation of benzyl alcohol on Au NPs readily occur,65,66 the low activity observed for Au/g-C3N4 suggests that the molecular oxygen is not being activated. That is, the Au NPs, as well as the g-C3N4, cannot activate the molecular oxygen in the reaction. Consequently, it is inferred that the molecular oxygen is only activated on the AC support, when Au/AC is used as catalyst. Similar results were also observed for CO+O2 reaction.64 Catalytic performances were investigated for benzyl alcohol oxidation reaction using Au NPs supported on AC with diﬀerent amounts of surface oxygen functional groups (SOFG), in order to investigate how molecular oxygen is activated on this support. The results show that the conversion of benzyl alcohol depends intimately on the amount of SOFG, as seen in Figure 10B,64 suggesting that the oxygen activation proceeds through the SOFG of AC. This is also supported by FT-IR and UV−vis measurements.67 It is therefore explained why Au NPs supported on g-C3N4 (i.e., Au/g-C3N4) show negligible activity, as g-C3N4 has no SOFG and hence no oxygen activation sites. An interesting work regarding the catalytic performances of Au and Pt NPs supported on carbon nitrides−silica composites (CNx/SBA-15) for CO+O2 reaction was recently reported.68 Although both metals have small particle size ( 420 nm) irradiation. (B) Cyclic runs of RhB (10 mM) degradation by H2O2 (0.05 M) activated by the Fe/g-C3N4 catalyst (40 mg). All reactions were carried out at neutral pH using the 10%-Fe/g-C3N4 catalyst. Reprinted with permission from ref 108. Copyright 2009 John Wiley & Sons.
Figure 18. (A) Visible-light-driven water oxidation by mpg-CNx-CoPi y% hybrid (y = 0, 1, 3, 5, and 10); (B) visible-light-driven hydrogen generation mediated by mpg-CNx-H2−CoCat photocatalyst, produced in situ from a mpg-CNx-H2−CoPi 10% composite, in a pH 7 phosphate buﬀer solution containing 10% (v/v) methanol; (C) visible-light-driven overall water splitting catalyzed by mpg-CNx-CoPi-H2−CoCat in pH 7 phosphate buﬀer solution without any scavengers.110 Reprinted with permission from ref 110. Copyright 2013 Royal Society of Chemistry.
Scheme 3. Schematic Diagram Showing the Process of (A) the Photocatalytic Dye Degradation over a g-C3N4−Ag3PO4 Compositea; (B) H2 Evolution Reaction over g-PAN/g-C3N4 Composites under Visible Light Irradiationb
Reprinted with permission from ref 111. Copyright 2013 Royal Society of Chemistry. bReprinted with permission from ref 112. Copyright 2014 American Chemical Society.
oxide-phosphate (CoPi) water oxidation material onto the surface of a mpg-CNx semiconductor.110 The mpg-CNx-CoPi hybrid can be evolved to mpg-CNx-H2−CoCat and subsequently to mpg-CNx−CoPi−H2−CoCat, after successive
reactions. In brief, the mpg-CNx-CoPi hybrid, active for water oxidation reaction, is gradually converted into an active hydrogen evolution reaction catalyst, mpg-CNx-H2−CoCat, when a hole scavenger, e.g. methanol, is used. The coexistence 16460
of mpg-CNx-CoPi and mpg-CNx-H2−CoCat results in the formation of a mpg-CNx−CoPi−H2−CoCat composite, which is active for the overall water splitting process, with reaction rates of 13.6 μmol gcat−1 h−1 and 6.6 μmol gcat−1 h−1 for H2 and O2 evolution, respectively. In each case (water oxidation into oxygen, hydrogen production or water splitting into hydrogen and oxygen), the corresponding catalyst shows a signiﬁcantly enhanced activity compared to the untreated mpg-C3N4 catalyst, as depicted in Figure 18. To decrease the recombination rate of photoinduced electron−hole pairs, a cocatalyst or other semiconductor materials can be loaded onto the surface of g-C3N4, to form a hybrid nanocomposite material, which can enhance the charge separation and photostability, due to their diﬀerentiated band positions. Both inorganic metal semiconductors and organic or polymer materials can be used to hybridize with gC3N4; but the synthesis and the role in the reaction can be diﬀerent. For the former, Shanker et al. report that the gC3N4−Ag3PO4 nanocomposite photocatalyst can be prepared by in situ deposition of Ag3PO4 nanoparticles on the surface of a g-C3N4 sheet.111 This composite shows improved photoactivity for the degradation of methyl orange under visible light irradiation, which is 5 and 3.5 times higher than pure g-C3N4 and Ag3PO4 respectively. Furthermore, the stability of Ag3PO4 can be greatly improved and the amount of silver eﬀectively reduced. It is possible that the enhanced activity is due to smaller Ag3PO4 particle size, high surface area of the composite, or more critically, that a synergistic eﬀect is induced between gC3N4 and Ag3PO4. The electrons and holes induced by the visible light irradiation at the valence band (VB) and conduction band (CB) of Ag3O4 and g-C3N4 can then move freely under certain conditions, improving the charge separation eﬃciency of the photoinduced electron−hole pair, as shown in Scheme 3A. This is also true for other composites such as g-C3N4−AgX,113 g-C3N4−TiO2,114 g-C3N4−ZnO,115 and g-C3N4−BiPO4.116 In the case of the polymer/g-C3N4 hybrid, the synthesis needs to be done more carefully, so that the precursor of the incorporated polymer will not react or interfere with the precursor of g-C3N4, during the synthesis process. Nevertheless, these composites are more interesting and applicable in practice, since they are cheap and environmentally friendly samples, and have the possibility to form nanosheet structured materials, with several advantages for photocatalysis, such as a large speciﬁc surface area, oﬀering more reactive sites, and short diﬀusion distance, decreasing the recombination rate of photogenerated charge carriers.117 A recent work from He and co-workers shows that a sheet-on-sheet g-PAN/g-C3N4 composite (where g-PAN is a graphitized polyacrylonitrile), which is entirely composed of environmentally friendly polymer materials, can be obtained by a facile one-step thermal condensation of PAN and melamine.112 Photocatalytic tests show that the H2 evolution rate increases from 0.7 μmol h−1 for the pristine g-C3N4, to 3.1 μmol h−1 for the 5.0 wt % g-PAN/gC3N4 composite, and can be further improved to 37 μmol h−1 when a small amount of Pt is introduced, that is, Pt/5.0 wt % gPAN/g-C3N4. It is proposed that the role of g-PAN in the reaction is to improve the interfacial charge transfer under visible light irradiation, e.g., transfer the photoinduced electrons from the CB of g-C3N4 to the Pt particles. That eﬃciently suppresses the recombination rate of the photogenarated charge-hole pairs and improves the catalytic activity, as illustrated in Scheme 3B.
5. CONCLUSIONS AND OUTLOOKS This work summarizes the synthesis methods, physicochemical properties and applications of graphitic carbon nitride, g-C3N4, in heterogeneous catalysis. As a polymeric material, g-C3N4 can be prepared by polycondensation of a variety of precursors containing C/N/H and even O elements, and fabricated with diﬀerent structures (bulk, supported, porous) and morphologies. The results of TGA measurements show that g-C3N4 can endure temperatures up to 600 °C and that the proﬁles are similar in inert or oxygen atmospheres, suggesting that g-C3N4 has high thermal stability and is inactive to oxygen. However, CO2-TPD proﬁles suggest that the surface basicity of g-C3N4 is signiﬁcantly aﬀected by heating atmosphere, although no appreciable change in the crystalline structure is observed. Regarding the applications in catalysis, g-C3N4 is not only a good basic and metal-free catalyst for a variety of reactions, as reported in previous literature, but also an adequate reference material for diﬀerentiating the sites for oxygen activation over supported catalysts, and an excellent functional material in preparing small and stable metal nanoparticles for catalytic purposes. In spite of the great achievements over the years, there are still many challenges in the applications of this material in catalysis. First, the structure stability and surface area of g-C3N4 need to be improved. It is known that g-C3N4 prepared by condensation route usually suﬀers from incomplete polycondensation, leading to diﬀerent structures/composites from batch to batch, and the surface area of such prepared g-C3N4 material is low, which diminishes its catalytic activity. Although g-C3N4 with improved surface area can be obtained by a template method, the surface morphology and properties could be destroyed due to the drastic conditions used during the template etching process. Thus, the search for better, milder, and more reversible procedures to synthesize g-C3N4 with improved surface area is of crucial importance. Second, the physicochemical properties of g-C3N4 need to be further explored. Although g-C3N4 has been shown to be a good catalyst for several reactions, its actual role is not clear. The understanding of the physicochemical properties of g-C3N4 and its inﬂuence on the catalytic activity thus need to be correlated, in order to better understand the reaction and optimize the material. Finally, the most crucial is to improve the catalytic eﬃciency of g-C3N4 in the reactions. g-C3N4 is a covalent compound and its contribution to the reactions consists in the donation of electrons to the substrate, which requires the splitting and subsequent formation of the covalent bond during the reaction. This process is not easy, because of the high energy required for the splitting of a covalent bond, making the electron donation process slow and leading to low reaction rates. Therefore, the increase in surface energy and/or surface basicity of g-C3N4 is essential, to accelerate the rate of electron donation. Apart from its role as a metal-free catalyst, it is also important to seek for new applications of g-C3N4 in catalysis, namely, as a functional material to graft metal nanoparticles in catalyst preparation, and as a reference material to produce catalysts to distinguish the oxygen activation sites. The ﬁnding of new uses should be based on the better understanding of the physicochemical properties of g-C3N4, which will undoubtedly widen its applications and lead to more exciting results. 16461
The manuscript was written with the contributions of all authors. All authors approved the ﬁnal version of the manuscript. Notes
The authors declare no competing ﬁnancial interests.
ACKNOWLEDGMENTS J.Z. is grateful to prof. Kongyong Liew at South-central University for Nationalities for his contribution in the composition of the manuscript. Financial support from the National Science Foundation of China (21203254), the Scientiﬁc Research Foundation for Returned Scholars, Ministry of Education of China (BZY11055), and the National Demonstration Center of Experimental Teaching on ethnical pharmacy, South-Central University for Nationalities is greatly acknowledged. S.A.C.C. is grateful to Fundaçaõ para a Ciência e Tecnologia for Investigador FCT grant.
(1) Cohen, M. L. Calculation of Bulk Moduli of Diamond and Zincblende Solids. Phys. Rev. B 1985, 32, 7988−7991. (2) Liu, A. Y.; Cohen, M. L. Prediction of New Low Compressibility Solids. Science 1989, 245, 841−842. (3) Liebig, J. Uber Einige Stickstoff - Verbindungen. Ann. Pharm. 1834, 10, 1−47. (4) Wang, X.; Blechert, S.; Antonietti, M. Polymeric Graphitic Carbon Nitride for Heterogeneous Photocatalysis. ACS Catal. 2012, 2, 1596−1606. (5) Thomas, A.; Fischer, A.; Goettmann, F.; Antonietti, M.; Muller, J. O.; Schlogl, R.; Carlsson, J. M. Graphitic Carbon Nitride Materials: Variation of Structure and Morphology and Their Use as Metal-Free Catalysts. J. Mater. Chem. 2008, 18, 4893−4908. (6) Su, F.; Antonietti, M.; Wang, X. Mpg-C3n4 as a Solid Base Catalyst for Knoevenagel Condensations and Transesterification Reactions. Catal. Sci. Technol. 2012, 2, 1005−1009. (7) Zhu, J. J.; Wei, Y. C.; Chen, W. K.; Zhao, Z.; Thomas, A. Graphitic Carbon Nitride as a Metal-Free Catalyst for No Decomposition. Chem. Commun. 2010, 46, 6965−6967. (8) Wang, X. C.; Maeda, K.; Thomas, A.; Takanabe, K.; Xin, G.; Carlsson, J. M.; Domen, K.; Antonietti, M. A Metal-Free Polymeric Photocatalyst for Hydrogen Production from Water under Visible Light. Nat. Mater. 2009, 8, 76−80. (9) Goettmann, F.; Thomas, A.; Antonietti, M. Metal-Free Activation CO2 by Mesoporous Graphitic Carbon Nitride. Angew. Chem., Int. Ed. 2007, 46, 2717−2720. (10) Huang, Z.; Li, F.; Chen, B.; Lu, T.; Yuan, Y.; Yuan, G. WellDispersed g-C3N4 Nanophases in Mesoporous Silica Channels and Their Catalytic Activity for Carbon Dioxide Activation and Conversion. Appl. Catal., B 2013, 136−137, 269−277. (11) Jin, X.; Balasubramanian, V. V.; Selvan, S. T.; Sawant, D. P.; Chari, M. A.; Lu, G. Q.; Vinu, A. Highly Ordered Mesoporous Carbon Nitride Nanoparticles with High Nitrogen Content: A Metal-Free Basic Catalyst. Angew. Chem., Int. Ed. 2009, 48, 7884−7887. (12) Zheng, Y.; Jiao, Y.; Chen, J.; Liu, J.; Liang, J.; Du, A.; Zhang, W.; Zhu, Z.; Smith, S. C.; Jaroniec, M.; Lu, G. Q.; Qiao, S. Z. Nanoporous [email protected] Metal-Free Electrocatalysts for Highly Efficient Oxygen Reduction. J. Am. Chem. Soc. 2011, 133, 20116− 20119. (13) Tian, J.; Ning, R.; Liu, Q.; Asiri, A. M.; Al-Youbi, A. O.; Sun, X. Three-Dimensional Porous Supramolecular Architecture from Ultrathin g-C3N4 Nanosheets and Reduced Graphene Oxide: Solution SelfAssembly Construction and Application as a Highly Efficient Metal16462
(33) Dong, F.; Wu, L.; Sun, Y.; Fu, M.; Wu, Z.; Lee, S. C. Efficient Synthesis of Polymeric g-C3N4 Layered Materials as Novel Efficient Visible Light Driven Photocatalysts. J. Mater. Chem. 2011, 21, 15171− 15174. (34) Zou, X.-X.; Li, G.-D.; Wang, Y.-N.; Zhao, J.; Yan, C.; Guo, M.Y.; Li, L.; Chen, J.-S. Direct Conversion of Urea into Graphitic Carbon Nitride over Mesoporous TiO2 Spheres under Mild Condition. Chem. Commun. 2011, 47, 1066−1068. (35) Dai, H.; Gao, X.; Liu, E.; Yang, Y.; Hou, W.; Kang, L.; Fan, J.; Hu, X. Synthesis and Characterization of Graphitic Carbon Nitride Sub-Microspheres Using Microwave Method under Mild Condition. Diamond Relat. Mater. 2013, 38, 109−117. (36) Lotsch, B. V.; Schnick, W. Thermal Conversion of Guanylurea Dicyanamide into Graphitic Carbon Nitride Via Prototype Cnx Precursors. Chem. Mater. 2005, 17, 3976−3982. (37) Lotsch, B. V.; Schnick, W. From Triazines to Heptazines: Novel Nonmetal Tricyanomelaminates as Precursors for Graphitic Carbon Nitride Materials. Chem. Mater. 2006, 18, 1891−1900. (38) Kroke, E.; Schwarz, M.; Horath-Bordon, E.; Kroll, P.; Noll, B.; Norman, A. D. Tri-S-Triazine Derivatives. Part I. From Trichloro-TriS-Triazine to Graphitic C3N4 Structures. New J. Chem. 2002, 26, 508− 512. (39) Matsumoto, S.; Xie, E. Q.; Izumi, F. On the Validity of the Formation of Crystalline Carbon Nitrides, C3N4. Diamond Relat. Mater. 1999, 8, 1175−1182. (40) Semencha, A. V.; Blinov, L. N. Theoretical Prerequisites, Problems, and Practical Approaches to the Preparation of Carbon Nitride: A Review. Glass Phys. Chem. 2010, 36, 199−208. (41) Bojdys, M. J. On New Allotropes and Nanostructures of Carbon Nitrides. Ph.D. Dissertation, Universitätsbibliothek Potsdam & MaxPlanck Institute of Colloids and Interfaces, Potsdam, Germany, 2009. (42) Zhang, Y. J.; Thomas, A.; Antonietti, M.; Wang, X. C. Activation of Carbon Nitride Solids by Protonation: Morphology Changes, Enhanced Ionic Conductivity, and Photoconduction Experiments. J. Am. Chem. Soc. 2009, 131, 50−51. (43) Goettmann, F.; Fischer, A.; Antonietti, M.; Thomas, A. MetalFree Catalysis of Sustainable Friedel-Crafts Reactions: Direct Activation of Benzene by Carbon Nitrides to Avoid the Use of Metal Chlorides and Halogenated Compounds. Chem. Commun. 2006, 4530−4532. (44) Wang, Y.; Li, H.; Yao, J.; Wang, X.; Antonietti, M. Synthesis of Boron Doped Polymeric Carbon Nitride Solids and Their Use as Metal-Free Catalysts for Aliphatic C-H Bond Oxidation. Chem. Sci. 2011, 2, 446−450. (45) Roeser, J.; Kailasam, K.; Thomas, A. Covalent Triazine Frameworks as Heterogeneous Catalysts for the Synthesis of Cyclic and Linear Carbonates from Carbon Dioxide and Epoxides. ChemSusChem 2012, 5, 1793−1799. (46) Wang, T.; Kailasam, K.; Xiao, P.; Chen, G.; Chen, L.; Wang, L.; Li, J.; Zhu, J. Adsorption Removal of Organic Dyes on Covalent Triazine Framework (CTF). Microporous Mesoporous Mater. 2014, 187, 63−70. (47) Pietrzak, R.; Wachowska, H.; Nowicki, P. Preparation of Nitrogen-Enriched Activated Carbons from Brown Coal. Energy Fuels 2006, 20, 1275−1280. (48) Grzybek, T.; Klinik, J.; Samojeden, B.; Suprun, V.; Papp, H. Nitrogen-Promoted Active Carbons as DeNO(x) Catalysts−1. The Influence of Modification Parameters on the Structure and Catalytic Properties. Catal. Today 2008, 137, 228−234. (49) Wang, Y.; Di, Y.; Antonietti, M.; Li, H.; Chen, X.; Wang, X. Excellent Visible-Light Photocatalysis of Fluorinated Polymeric Carbon Nitride Solids. Chem. Mater. 2010, 22, 5119−5121. (50) Liu, G.; Niu, P.; Sun, C.; Smith, S. C.; Chen, Z.; Lu, G. Q.; Cheng, H.-M. Unique Electronic Structure Induced High Photoreactivity of Sulfur-Doped Graphitic C3N4. J. Am. Chem. Soc. 2010, 132, 11642−11648. (51) Zhang, Y.; Mori, T.; Ye, J.; Antonietti, M. Phosphorus-Doped Carbon Nitride Solid: Enhanced Electrical Conductivity and Photocurrent Generation. J. Am. Chem. Soc. 2010, 132, 6294−6295.
(52) Zhu, J. J.; Thomas, A. Perovskite-Type Mixed Oxides as Catalytic Material for NO Removal. Appl. Catal,. B 2009, 92, 225−233. (53) Zhu, J. J.; Mao, D. H.; Li, J.; Xie, X. F.; Yang, X. G.; Wu, Y. Recycle - New Possible Mechanism of No Decomposition over Perovskite(-Like) Oxides. J. Mol. Catal. A: Chem. 2005, 233, 29−34. (54) Zhu, J. J.; Yang, X. G.; Xu, X. L.; Wei, K. M. Active Site Structure of No Decomposition on Perovskite(-Like) Oxides: An Investigation from Experiment and Density Functional Theory. J. Phys. Chem. C 2007, 111, 1487−1490. (55) Sokolovskii, V. D. Principles of Oxidative Catalysis on Solid Oxides. Catal. Rev. 1990, 32, 1−49. (56) Schubert, M. M.; Hackenberg, S.; van Veen, A. C.; Muhler, M.; Plzak, V.; Behm, R. J. CO Oxidation over Supported Gold Catalysts″Inert″ and ″Active″ Support Materials and Their Role for the Oxygen Supply During Reaction. J. Catal. 2001, 197, 113−122. (57) Yan, Z.; Chinta, S.; Mohamed, A. A.; Fackler, J. P.; Goodman, D. W. The Role of F-Centers in Catalysis by Au Supported on MgO. J. Am. Chem. Soc. 2005, 127, 1604−1605. (58) Haruta, M.; Date, M. Advances in the Catalysis of Au Nanoparticles. Appl. Catal. A-Gen. 2001, 222, 427−437. (59) Liu, H.; Kozlov, A. I.; Kozlova, A. P.; Shido, T.; Asakura, K.; Iwasawa, Y. Active Oxygen Species and Mechanism for LowTemperature CO Oxidation Reaction on a TiO2-Supported Au Catalyst Prepared from Au(PPh3)(NO3) and as-Precipitated Titanium Hydroxide. J. Catal. 1999, 185, 252−264. (60) Okumura, M.; Coronado, J. M.; Soria, J.; Haruta, M.; Conesa, J. C. EPR Study of CO and O2 Interaction with Supported Au Catalysts. J. Catal. 2001, 203, 168−174. (61) Liu, Z. P.; Gong, X. Q.; Kohanoff, J.; Sanchez, C.; Hu, P. Catalytic Role of Metal Oxides in Gold-Based Catalysts: A First Principles Study of CO Oxidation on TiO2 Supported Au. Phys. Rev. Lett. 2003, 91, 266102−266105. (62) Haruta, M. Catalysis−Gold Rush. Nature 2005, 437, 1098− 1099. (63) Widmann, D.; Behm, R. J. Activation of Molecular Oxygen and the Nature of the Active Oxygen Species for CO Oxidation on Oxide Supported Au Catalysts. Acc. Chem. Res. 2014, 47, 740−749. (64) Zhu, J. J.; Carabineiro, S. A. C.; Shan, D.; Faria, J. L.; Zhu, Y. J.; Figueiredo, J. L. Oxygen Activation Sites in Gold and Iron Catalysts Supported on Carbon Nitride and Activated Carbon. J. Catal. 2010, 274, 207−214. (65) Mallat, T.; Baiker, A. Oxidation of Alcohols with Molecular Oxygen on Solid Catalysts. Chem. Rev. 2004, 104, 3037−3058. (66) Corma, A.; Garcia, H. Supported Gold Nanoparticles as Catalysts for Organic Reactions. Chem. Soc. Rev. 2008, 37, 2096−2126. (67) Zhu, J. J.; Faria, J. L.; Figueiredo, J. L.; Thomas, A. Reaction Mechanism of Aerobic Oxidation of Alcohols Conducted on Activated-Carbon-Supported Cobalt Oxide Catalysts. Chem.Eur. J. 2011, 17, 7112−7117. (68) Xiao, P.; zhao, Y. X.; Wang, T.; Zhan, Y. Y.; Wang, H. H.; Li, J. L.; Thomas, A.; Zhu, J. J. Polymeric Carbon Nitride/Mesoporous Silica Composites as Catalyst Support for Au and Pt Nanoparticles. Chem.Eur. J. 2014, 20, 2872−2878. (69) Turner, M.; Golovko, V. B.; Vaughan, O. P. H.; Abdulkin, P.; Berenguer-Murcia, A.; Tikhov, M. S.; Johnson, B. F. G.; Lambert, R. M. Selective Oxidation with Dioxygen by Gold Nanoparticle Catalysts Derived from 55-Atom Clusters. Nature 2008, 454, 981−984. (70) Zhu, Y.; Zaera, F. Selectivity in the Catalytic Hydrogenation of Cinnamaldehyde Promoted by Pt/SiO2 as a Function of Metal Nanoparticle Size. Catal. Sci. Technol. 2014, 4, 955−962. (71) Lee, I.; Delbecq, F.; Morales, R.; Albiter, M. A.; Zaera, F. Tuning Selectivity in Catalysis by Controlling Particle Shape. Nat. Mater. 2009, 8, 132−138. (72) Prashar, A. K.; Mayadevi, S.; Nandini Devi, R. Effect of Particle Size on Selective Hydrogenation of Cinnamaldehyde by Pt Encapsulated in Mesoporous Silica. Catal. Commun. 2012, 28, 42−46. (73) Alivisatos, A. P. Semiconductor Clusters, Nanocrystals, and Quantum Dots. Science 1996, 271, 933−937. 16463
(74) Zhu, J.; Wang, T.; Xu, X.; Xiao, P.; Li, J. Pt Nanoparticles Supported on SBA-15: Synthesis, Characterization and Applications in Heterogeneous Catalysis. Appl. Catal., B 2013, 130−131, 197−217. (75) Lee, B.; Ma, Z.; Zhang, Z.; Park, C.; Dai, S. Influences of Synthesis Conditions and Mesoporous Structures on the Gold Nanoparticles Supported on Mesoporous Silica Hosts. Microporous Mesoporous Mater. 2009, 122, 160−167. (76) Konova, P.; Naydenov, A.; Venkov, C.; Mehandjiev, D.; Andreeva, D.; Tabakova, T. Activity and Deactivation of Au/TiO2 Catalyst in Co Oxidation. J. Mol. Catal. A: Chem. 2004, 213, 235−240. (77) Chan-Thaw, C. E.; Villa, A.; Katekomol, P.; Su, D. S.; Thomas, A.; Prati, L. Covalent Triazine Framework as Catalytic Support for Liquid Phase Reaction. Nano Lett. 2010, 10, 537−541. (78) Yang, C.-m.; Kalwei, M.; Schüth, F.; Chao, K.-j. Gold Nanoparticles in SBA-15 Showing Catalytic Activity in CO Oxidation. Appl. Catal., A 2003, 254, 289−296. (79) Joo, S. H.; Park, J. Y.; Tsung, C.-K.; Yamada, Y.; Yang, P.; Somorjai, G. A. Thermally Stable Pt/Mesoporous Silica Core-Shell Nanocatalysts for High-Temperature Reactions. Nat. Mater. 2009, 8, 126−131. (80) Chan-Thaw, C. E.; Villa, A.; Prati, L.; Thomas, A. TriazineBased Polymers as Nanostructured Supports for the Liquid-Phase Oxidation of Alcohols. Chem.Eur. J. 2011, 17, 1052−1057. (81) Chan-Thaw, C. E.; Villa, A.; Veith, G. M.; Kailasam, K.; Adamczyk, L. A.; Unocic, R. R.; Prati, L.; Thomas, A. Influence of Periodic Nitrogen Functionality on the Selective Oxidation of Alcohols. Chem.Asian J. 2012, 7, 387−393. (82) Li, Y.; Xu, X.; Zhang, P.; Gong, Y.; Li, H.; Wang, Y. Highly Selective [email protected] Catalyst for Phenol Hydrogenation in Aqueous Phase. RSC Adv. 2013, 3, 10973−10982. (83) Li, Y.; Gong, Y.; Xu, X.; Zhang, P.; Li, H.; Wang, Y. A Practical and Benign Synthesis of Amines through [email protected] Catalyzed Reduction of Nitriles. Catal. Commun. 2012, 28, 9−12. (84) Wang, Y.; Yao, J.; Li, H.; Su, D.; Antonietti, M. Highly Selective Hydrogenation of Phenol and Derivatives over a [email protected] Nitride Catalyst in Aqueous Media. J. Am. Chem. Soc. 2011, 133, 2362−2365. (85) Deng, D.; Yang, Y.; Gong, Y.; Li, Y.; Xu, X.; Wang, Y. Palladium Nanoparticles Supported on mpg-C3N4 as Active Catalyst for Semihydrogenation of Phenylacetylene under Mild Conditions. Green Chem. 2013, 15, 2525−2531. (86) Chang, C.; Fu, Y.; Hu, M.; Wang, C.; Shan, G.; Zhu, L. Photodegradation of Bisphenol a by Highly Stable Palladium-Doped Mesoporous Graphite Carbon Nitride (Pd/mpg-C3N4) under Simulated Solar Light Irradiation. Appl. Catal., B 2013, 142−143, 553−560. (87) Li, X.-H.; Wang, X.; Antonietti, M. Mesoporous g-C3N4 Nanorods as Multifunctional Supports of Ultrafine Metal Nanoparticles: Hydrogen Generation from Water and Reduction of Nitrophenol with Tandem Catalysis in One Step. Chem. Sci. 2012, 3, 2170−2174. (88) Cui, Y.; Ding, Z.; Liu, P.; Antonietti, M.; Fu, X.; Wang, X. Metalfree Activation of H2O2 by g-C3N4 under Visible Light Irradiation for the Degradation of Organic Pollutants. Phys. Chem. Chem. Phys. 2012, 14, 1455−1462. (89) Cheng, N.; Tian, J.; Liu, Q.; Ge, C.; Qusti, A. H.; Asiri, A. M.; Al-Youbi, A. O.; Sun, X. Au-Nanoparticle-Loaded Graphitic Carbon Nitride Nanosheets: Green Photocatalytic Synthesis and Application toward the Degradation of Organic Pollutants. ACS Appl. Mater. Interfaces 2013, 5, 6815−6819. (90) Chang, C.; Zhu, L.; Wang, S.; Chu, X.; Yue, L. Novel Mesoporous Graphite Carbon Nitride/BiOI Heterojunction for Enhancing Photocatalytic Performance Under Visible-Light Irradiation. ACS Appl. Mater. Interfaces 2014, 6, 5083−5093. (91) Lewis, N. S.; Nocera, D. G. Powering the planet: Chemical challenges in solar energy utilization. Proc. Natl. Acad. Sci. U.S.A. 2006, 103, 15729−15735. (92) Cook, T. R.; Dogutan, D. K.; Reece, S. Y.; Surendranath, Y.; Teets, T. S.; Nocera, D. G. Solar Energy Supply and Storage for the Legacy and Nonlegacy Worlds. Chem. Rev. 2010, 110, 6474−6502.
(93) Liu, J.; Zhang, Y.; Lu, L.; Wu, G.; Chen, W. Self-regenerated Solar-driven Pphotocatalytic Water-splitting by Urea Derived Graphitic Carbon Nitride with Platinum Nanoparticles. Chem. Commun. 2012, 48, 8826−8828. (94) Mao, J.; Peng, T.; Zhang, X.; Li, K.; Ye, L.; Zan, L. Effect of Graphitic Carbon Nitride Microstructures on the Activity and Selectivity of Photocatalytic CO2 Reduction under Visible Light. Catal. Sci. Technol. 2013, 3, 1253−1260. (95) Lin, J.; Pan, Z.; Wang, X. Photochemical Reduction of CO2 by Graphitic Carbon Nitride Polymers. ACS Sustainable Chem. Eng. 2013, 2, 353−358. (96) Zhang, P.; Gong, Y.; Li, H.; Chen, Z.; Wang, Y. Selective Oxidation of Benzene to Phenol by FeCl3/mpg-C3N4 Hybrids. RSC Adv. 2013, 3, 5121−5126. (97) Wang, X.; Maeda, K.; Thomas, A.; Takanabe, K.; Xin, G.; Carlsson, J. M.; Domen, K.; Antonietti, M. A Metal-free Polymeric Photocatalyst for Hydrogen Production from Water under Visible Light. Nat. Mater. 2009, 8, 76−80. (98) Maeda, K.; Wang, X.; Nishihara, Y.; Lu, D.; Antonietti, M.; Domen, K. Photocatalytic Activities of Graphitic Carbon Nitride Powder for Water Reduction and Oxidation under Visible Light. J. Phys. Chem. C 2009, 113, 4940−4947. (99) Wang, X.; Maeda, K.; Chen, X.; Takanabe, K.; Domen, K.; Hou, Y.; Fu, X.; Antonietti, M. Polymer Semiconductors for Artificial Photosynthesis: Hydrogen Evolution by Mesoporous Graphitic Carbon Nitride with Visible Light. J. Am. Chem. Soc. 2009, 131, 1680−1681. (100) Zhang, M.; Xu, J.; Zong, R.; Zhu, Y. Enhancement of Visible Light Photocatalytic Activities via Porous Structure of g-C3N4. Appl. Catal,. B 2014, 147, 229−235. (101) Xu, J.; Wang, Y.; Zhu, Y. Nanoporous Graphitic Carbon Nitride with Enhanced Photocatalytic Performance. Langmuir 2013, 29, 10566−10572. (102) Cui, Y.; Huang, J.; Fu, X.; Wang, X. Metal-free Photocatalytic Degradation of 4-Chlorophenol in Water by Mesoporous Carbon Nitride Semiconductors. Catal. Sci. Technol. 2012, 2, 1396−1402. (103) Li, J.; Shen, B.; Hong, Z.; Lin, B.; Gao, B.; Chen, Y. A Facile Approach to Synthesize Novel Oxygen-doped g-C3N4 with Superior Visible-light Photoreactivity. Chem. Commun. 2012, 48, 12017−12019. (104) Dong, G.; Zhao, K.; Zhang, L. Carbon Self-doping Induced High Electronic Conductivity and Photoreactivity of g-C3N4. Chem. Commun. 2012, 48, 6178−6180. (105) Zhang, J.; Sun, J.; Maeda, K.; Domen, K.; Liu, P.; Antonietti, M.; Fu, X.; Wang, X. Sulfur-mediated Synthesis of Carbon Nitride: Band-gap Engineering and Improved Functions for Photocatalysis. Energy Environ. Sci. 2011, 4, 675−678. (106) Yan, S. C.; Li, Z. S.; Zou, Z. G. Photodegradation of Rhodamine B and Methyl Orange over Boron-Doped g-C3N4 under Visible Light Irradiation. Langmuir 2010, 26, 3894−3901. (107) Zhang, G.; Zhang, J.; Zhang, M.; Wang, X. Polycondensation of Thiourea into Carbon Nitride Semiconductors as Visible Light Photocatalysts. J. Mater. Chem. 2012, 22, 8083−8091. (108) Wang, X.; Chen, X.; Thomas, A.; Fu, X.; Antonietti, M. MetalContaining Carbon Nitride Compounds: A New Functional Organic− Metal Hybrid Material. Adv. Mater. 2009, 21, 1609−1612. (109) Gao, H.; Yan, S.; Wang, J.; Zou, Z. Ion Coordination Significantly Enhances the Photocatalytic Activity of Graphitic-phase Carbon Nitride. Dalton. Trans. 2014, 43, 8178−8183. (110) Lee, R.-L.; Tran, P. D.; Pramana, S. S.; Chiam, S. Y.; Ren, Y.; Meng, S.; Wong, L. H.; Barber, J. Assembling Graphitic-CarbonNitride with Cobalt-Oxide-Phosphate to Construct an Efficient Hybrid Photocatalyst for Water Splitting Application. Catal. Sci. Technol. 2013, 3, 1694−1698. (111) Kumar, S.; Surendar, T.; Baruah, A.; Shanker, V. Synthesis of a Novel and Stable g-C3N4-Ag3PO4 Hybrid Nanocomposite Photocatalyst and Study of the Photocatalytic Activity under Visible Light Irradiation. J. Mater. Chem. A 2013, 1, 5333−5340. (112) He, F.; Chen, G.; Yu, Y.; Hao, S.; Zhou, Y.; Zheng, Y. Facile Approach to Synthesize g-PAN/g-C3N4 Composites with Enhanced 16464